development of advanced cores and castings for .investment casting institute maughan and thompson,
Post on 19-Jun-2019
Embed Size (px)
Investment Casting Institute
65th Technical Conference and Expo
October 21-24, 2018, Kansas City, MO.
DEVELOPMENT OF ADVANCED CORES AND CASTINGS
FOR IMPROVED GAS TURBINE PERFORMANCE
James R. Maughan, PhD
Schenectady Cores and Castings
Schenectady, NY, USA
A. Mark Thompson, PhD
GE Global Research
Materials and Manufacturing Technology
Schenectady, NY, USA
Perhaps the most significant design challenge in a modern gas turbine is
maintaining adequate life of the high-temperature blades without sacrificing performance
through excessive cooling air. This optimization requires tight integration between the
mechanical, aerodynamic, and thermal design of the blade and the manufacturing
constraints of the ceramic core and superalloy investment casting process. One turbine
manufacturer has recently completed a facility to develop and manufacture advanced,
high-performance ceramic cores, validate these cores in the casting process, produce cores
at scale, and produce castings at pilot scale.
This paper describes the three-dimensional, complex design features of low-flow
ceramic cores and discusses some of the related manufacturing implications for the cores
and castings. An overview of the production facility will be given, including ceramic core
processing, methods to adapt single crystal investment casting to these complex
geometries, and new inspection techniques involving high-powered computed tomography.
Lastly, examples will be shown of the techniques and advantages to cycle and yield of
modeling, including grain growth, microstructure, core shift, and residual stresses.
As gas turbine efficiency increases significantly with turbine inlet temperature,
design requirements of the first stage turbine blade have become increasingly challenging.
Turbine inlet temperatures in the newest machines are several hundred degrees higher than
the melting point of nickel-based super alloys from which the hot gas path components are
cast. These components operate with a three year service interval and achieve that design
Investment Casting Institute Maughan and Thompson, GE Power p. 2
life through single crystal, creep-resistant
metallurgy, dense vertically-cracked thermal
barrier coatings, shaped-hole film cooling, and
internal turbulated cooling passages (Figure 1).
Cooling air used inside the blade does not
produce useful work in that turbine row and
therefore significantly reduces turbine output
and efficiency. Designers are constantly seeking
to decrease the amount and increase the
effectiveness of that cooling air.
CERAMIC CORES FOR ADVANCED BLADE COOLING
The ceramic cores used in the investment casting process to create internal cooling
passages are themselves subject to design and manufacturing constraints. These cores are
conventionally produced by injection of a ceramic
slurry into a hard-tooled metal die, with subsequent
firing and finishing processes. The die design
requirement of a single pull plane or a reasonable
number of slides restricts the design options for the
internal cooling passages, typically resulting in a
fairly simple internal structure similar to that shown
in Figure 2. While this configuration will pass a
significant amount of air through the blade, it is
evident that a limited fraction of the cooling air is
directly against the hot surface of the metal, and much of the air is wasted passing through
the interior of the blade, despite the mitigating strategy of serpentine passages, with flow
up one passage and down another.
Designers have long envisioned more complex internal structures such as that
Figure 1. Finished gas turbine blade
manufactured as an investment casting with a
ceramic core to form internal cooling channels.
Figure 2. Cross section of gas turbine
blade with conventional internal cooling.
Investment Casting Institute Maughan and Thompson, GE Power p. 3
shown in Figure 31, where the lowest temperature
cooling air can be restricted to the hottest internal
surfaces of the blade, and leave the center of the blade
stagnant or for the return of spent air. In such a manner,
the same blade temperature can be achieved with lower
cooling air flow, a cooler blade can be achieved with
the same flow, or a higher gas path temperature can be
achieved with the same flow and the same blade
temperature. In any of these applications of Advanced
Blade Cooling (ABC), there is a significant benefit to overall machine performance. The
gas turbine industry has spent significant effort attempting to develop the design and
manufacturing technology needed to produce the ABC ceramic cores required to cast these
complex shapes.2 3 4
One such ceramic core resulting from that research is shown in Figure 4 and the
corresponding blade in Figure 5. Volume production of these components is part of the GE
7HA.02 product line.5 While details of the specific manufacturing technologies involved
are not relevant to this summary of its impact on investment casting development and
application, the process is not constrained by conventional dies and hard tooling, thereby
improving the designers ability to optimize performance. Overcoming the technical issues
created by removing these limitations, however, has taken nearly a decade of research and
Figure 3. Schematic of cross section
showing Advanced Blade Cooling.
Figure 5. Single crystal blade cast with an ABC core. Figure 4. ABC ceramic core.
Investment Casting Institute Maughan and Thompson, GE Power p. 4
DESIGN AND APPLICATION CONSIDERATIONS
The development of these cores necessitated close integration with the design
process for air-cooled gas turbine blades. External aerodynamics are unaffected by the
advanced cores, as this was an early design constraint. In some cases, existing analysis
tools for internal flow and heat transfer were modified to account for new flow geometries,
including turbulators, pins, flow splits, and film cooling hole inlet conditions. Mechanical
design is affected through the impact of the internal shape on response frequencies and
magnitudes, as well as the complexity of managing fatigue and life of the internal metal
structure under transient conditions.
Considerable effort was required to engineer a ceramic that is capable of being
precisely formed to these complex shapes, but that is also compatible with subsequent
ceramic firing and finishing and with the casting process itself. The complex geometry and
large variations in characteristic dimensions require shrinkage rates, composition, and
firing cycle to be optimized to minimize cracking while maintaining dimensions and
strength, a design challenge assisted by drawing from the depth of the manufacturers
expertise in ceramics processing and ceramic matrix composites. The ceramic composition,
firing stages, and fixture strategy acting together create a system that produces a repeatable
and dimensionally-stable process.
A further development objective was to minimize the need for changes to the single
crystal casting process, and to adapt the advanced core design to make subsequent casting
and post-cast process comparable for blades with either conventional cores or advanced
cores, as demonstrated through casting trials. The core material is slightly stronger than
conventional serpentine cores and thus has good yield through wax pattern injection but is
not so strong that it causes internal stresses that lead
to recrystallization. Thermal expansion
characteristics at casting temperature are similar to
conventional cores, and thus the material can be used
with the same shelling system and slip techniques
familiar in the industry today. Some consideration
had to be given to internal core supports, pinning
locations, core bonding, reducing porosity at
Figure 6. Micrograph of interface
between core and cast alloy.
Investment Casting Institute Maughan and Thompson, GE Power p. 5
turnarounds, managing residual stress, and leaching. Detailed micrography has confirmed
that the interaction between the core and the alloy is similar to that expected for a high
silica core (Figure 6).
The resultant ABC core has characteristics similar enough to conventional
serpentine cores used today that it can be cast and leached via conventional processes,
leaving behind the complex cooling channels in the airfoil. Internal and external casting
trials have validated the ceramic core technology is mature to the point where it can be cast
across multiple foundries with minimal changes to existing casting processes.
An additional significant consideration in the application of these three-
dimensional, multi-wall cores is inspectability.
Borescope access to every internal region of the